# Analysis of Fatigue Fracture of Tank Wagon Railway of Fatigue Fracture of Tank Wagon Railway Axles ... to fracture of tank wagon railway ... used by AFGROW is a closed form solution,

Post on 06-Feb-2018

216 views

Embed Size (px)

TRANSCRIPT

Analysis of Fatigue Fracture of Tank Wagon Railway Axles

COSMIN LOCOVEI cosmin.locovei@mec.upt.ro

AUREL RDU

aurel.raduta@mec.upt.ro

MIRCEA NICOAR mircea.nicoara@mec.upt.ro

LAURENIU ROLAND CUCURUZ

roland.cucuruz@mec.upt.ro Department of Materials and Manufacturing Engineering,

POLITEHNICA University of Timioara Bd. M. Viteazul 1, 300222 Timioara,

ROMANIA

Abstract: - The paper is focused on the fracture mechanism of railway axles due to the fatigue of material. The purpose of the present article is to numerically predict the number of cycles (or kilometers) to fracture of tank wagon railway axles in various theoretical conditions. The stresses in the axles were calculated by finite element methods. The number of cycles to fracture was calculated using closed form solution of NASGRO equation for fatigue crack development starting from an initial crack detectable by means of non-destructive testing. In order to demonstrate the deep negative impact of forbidden thermal treatments and operations applied to railway axles, residual stresses of these treatments were calculated and new numerical predictions of number of cycles to fracture have been made.

Key-Words: - fatigue fracture, NASGRO equation (FormanNewmande Koning equation), von Misses stresses, residual stresses, finite element analysis (FEA).

1 Introduction Lately, an unprecedented series of major railway axle fractures with many similarities have occurred. All broken axles were from gasoline tank wagons with a relatively massive load compared to the load of passenger wagons. All broken axles were fractured due to the fatigue of material as seen in figure 1 and were manufactured by the same company in the same month.

Figure 1. Broken tank wagon axle from a severe derailment.

The fracture of the axles has occurred in the area of most intense stresses, below the locking ring (represented in blue) of the bearing (represented in green), as seen in figure 2.

Figure 2. Simpified 3D representation of an railway

axle.

In some cases, after the fracture, the wagon continued to run with all the load of the axle supported by the bearing box (represented in red). The heat produced by the

Proceedings of the 3rd WSEAS Int. Conference on FINITE DIFFERENCES - FINITE ELEMENTS - FINITE VOLUMES - BOUNDARY ELEMENTS

ISSN: 1790-2769 219 ISBN: 978-960-474-180-9

intense friction of the axle and the locking ring against the bearing box (figure 3) causes the melt of the locking ring and, ultimately of the bearing box (figure 4 and 5). After the fracture of the axle, the locking ring of the bearing and the axle continues to jointly rotate, as the locking ring is still suporting the load of the wagon through the bearing box. The load is distributed on a small area of the surface of bearing box and of the locking ring (figure 3).

Figure 3. 3D simplified representation of friction of the

locking ring against bearing box.

Figure 4. 3D simplified representation of the channel

formed as an effect of heat disipated in the bearing box.

Consequently the heat resulting from the friction is distributed on a small volume of material, causing a rapid augmentation of the temperature. The elevated temperatures cause the decrease of mechanical properties of the material of the bearing box, that lead to the deformation and fracture of bearing box. The purpose of this article is to numerically simulate the loads, stresses and predict the number of cycles (or kilometers) to fracture in various theoretical conditions. This article does not substitute in any way the legal inquiries (still pending at the time of this article being

written) and does not make any assumption or statement regarding the accidents.

Figure 5. The fracture of bearing box as a result of heat

disipated from friction against the locking ring.

2 Methods An accurate 3D model of the axle has been created using mechanical design software as in figure 6. Restraints and static loads have been applied to this model, in order to numerically calculate von Misses stresses. No translation type restraints have been applied to cylindrical surfaces that connect the railway axle to the wheels. The maximum load of 100 kN has been applied on both ends of the axle. After meshing of the 3D model, a static analysis has been performed and von Misses stresses have been calculated. Maximum von Misses stresses were of 86.27 MPa that is very low in comparison with yield strength of the A1N steel. The deformation scale in figure 7 is 1416.9. The mechanical properties of the material are shown in Table 1.

Table 1. Mechanical properties of A1N steel. Mechanical Properties of

A1N steel Value

Elastic Modulus 210000 N/m Poissons Ratio 0.26 Shear Modulus 78000 N/m2

Density 7300 kg/m3 Ultimate Tensile Strength 550 N/mm2

Compression Strength 550 N/mm2 Yield Strength 350 N/mm2

Thermal Expansion Coefficient 1.510

-5/Kelvin

Thermal Conductivity 38 W/(m.K) Specific Heat 440 J/(kg.K)

Mechanical Properties of A1N steel

Value

Proceedings of the 3rd WSEAS Int. Conference on FINITE DIFFERENCES - FINITE ELEMENTS - FINITE VOLUMES - BOUNDARY ELEMENTS

ISSN: 1790-2769 220 ISBN: 978-960-474-180-9

In order to ensure a much more realistic estimation of stresses in the axle, the dynamic loads have been taken into consideration as a static model [2]. We have found the maximum von Misses stresses to be 110.7 MPa, a value that is three times lower than the yield strength.

Figure 6. 3D CAD model of the tank wagon railway

axle.

Figure 7. Von Misses stresses and deformations for a

tank wagon railway axle model. In order to apply the worse case scenario further fracture analyses have been completed right in the section of the axle with maximum von Misses stresses. In addition, other simulations are proposed using residual stresses from a theoretical 5 mm depth welded layer (even if such mechanical operations are strictly prohibited by railway regulation). In fact, in railway industry, if a structural moving part does not meet the required dimensions or has material defects (like scratches or cracks) it is strictly forbidden to cover or repair the part using welding or any other heat treatment). These additional simulations were made in order to highlight the real risks of such a procedure. Fracture analyses were completed using NASGRO equation (Eq. 1),

expression also called FormanNewmande Koning equation jointly introduced by NASA and ESA [2], which is now common in aerospace applications. Equation 1 was numerically solved using AFGROW software.

q

Jc

p

effneff

K

K

K

K

KCdN

da

=

max

0

1

1

)( (eq. 1)

The numerical issues involved in crack propagation were further discussed in recent article [3]. The method used by AFGROW is a closed form solution, in this particular case; classic model of rod standard solution has been used. The methods in this paper are following the guidelines in recent articles [4] and [5].

3 Results During AFGROW crack growth simulation the following constants and mechanical material properties were used: Young's Modulus =206843 Poisson's Ratio =0.33 Coeff. of Thermal Expan. =1.26e-005 The Forman-Newman-de Koning- Henriksen (NASGRO) crack growth relation is being used No crack growth retardation is being considered For Reff < 0.0, Delta K = Kmax Material: A1N Plane strain fracture toughness: 76.919 Plane stress fracture toughness: 115.379 Effective fracture toughness for surface/elliptically shaped crack: 109.884 Fit parameters (KC versus Thickness Equation): Ak= 0.75, Bk=0.5 Yield stress: 350 Lower 'R' value boundary: -0.3 Upper 'R' value boundary: 0.8 Exponents in NASGRO Equation: n=3.6, p=0.5, q=0.5 Paris crack growth rate constant: 1.4473e-012 Threshold stress intensity factor range at R = 0: 8.791 Threshold coefficient: 2 Plane stress/strain constraint factor: 2.5 Ratio of the maximum applied stress to the flow stress: 0.5 Failure is based on the current load in the applied spectrum Vroman integration at 1% crack length A normalized spectrum has been used (figure 8) statistically reproducing the track with straight and curved segments of railway. The spectrum has been repeated until fracture has occurred. The load and the

Proceedings of the 3rd WSEAS Int. Conference on FINITE DIFFERENCES - FINITE ELEMENTS - FINITE VOLUMES - BOUNDARY ELEMENTS

ISSN: 1790-2769 221 ISBN: 978-960-474-180-9

initial crack were applied in the section of the axle with maximum stresses. The following results have been obtained after running the prediction of crack propagation as in Table 2 and figure 9.

Figure 8. Statistically determined normalized load

spectrum.

Figure 5. Predictions of crack c lengths [m] against number of cycles for a tank wagon railway axle with no

residual stresses starting from different initial crack sizes.

Table 2. Prediction as number of cycles and kilometers to failure for a tank wagon railway axle fracture with no

residual stresses Initial crack size c [mm]

4.5 6 7.5

Cycles to fracture (no residual stress)

- 6.1107 1.8107

Kilometers to fracture (no residual stress)

- 354000 109000

Let assumes that a 5 mm welded layer is laid on external surface of the axle including the section with most elevated stresses. Due to the thermal contraction some residual stresses will appear after the welded layer will cool down. As it was previously calculated in [5], the residual stresses can be determined with equation 2 and are plotted in figure 10.

amb

ambamb xTR

Recommended